RSC Article Template (Version 3.2)
Synthesis and self-assembly of amphiphilic polymers based on polyoxazoline and vegetable oil derivativesMylne Stemmelen,a Christophe Travelet,b Vincent Lapinte,*a Redouane Borsalib and Jean-Jacques Robina
Received 10th October 2012, Accepted 21th November 2012DOI: 10.1039/c2py20840gThe synthesis and self-assembly of amphiphilic polymers based on unsaturated vegetable oils and poly(2-methyl-2-oxazoline) (POx) are reported. Two architectures of lipopolymers were explored starting from fatty methyl esters and raw vegetable oils. These latter were converted into macroinitiators for cationic ring-opening polymerization (CROP) of 2-methyl-2-oxazoline. Firstly, a thiol-ene coupling reaction in the presence of mercaptoethanol under UV irradiation was performed to introduce hydroxyl groups that were further transformed into initiating species used for cationic polymerization. According to this strategy, various lipopoly(2-methyl-2-oxazoline)s (LipoPOx)s with different lipidic/POx ratios were successfully obtained and characterized by 1H NMR, SEC and MALDI-Tof analyses. Finally, the self-organization of the LipoPOx was studied using dynamic light scattering (DLS). Well-shaped nanoparticles were obtained with characteristic radii of 4.3 and 10.2 nm for the fatty ester- and triglyceride-based lipopolymers, respectively. The latter value is about twice the former one due to the higher lipidic fraction of the triglyceride-based polymer that promotes hydrophobic interactions. The relaxation time distributions of both systems were found to be monomodal indicating monodisperse colloidal suspensions.Polymer Chemistry
Dynamic Article LinksARTICLE TYPE
CREATED USING THE RSC ARTICLE TEMPLATE (VER. 3.0) - SEE WWW.RSC.ORG/ELECTRONICFILES FOR DETAILSARTICLE TYPEwww.rsc.org/xxxxxx | XXXXXXXXJournal NameCite this: DOI: 10.1039/c0xx00000xwww.rsc.org/xxxxxxDynamic Article LinksARTICLE TYPE
This journal is The Royal Society of Chemistry [year][Polym. Chem.], , , 14451458 |110|Journal Name, [year], [vol], 0000This journal is The Royal Society of Chemistry [year]This journal is The Royal Society of Chemistry [year]Journal Name, [year], [vol], 0000 |9INTRODUCTION As a consequence of the depleting of fossil reserves and environmental issues, the use of renewable raw materials is important for sustainable development1. The main bio-based raw materials are vegetable oils, polysaccharides, sugars and woods2 that are chemically modified for the development of chemicals, polymers2, amphiphilic copolymers, composites, blends3, plasticizers4, and coatings5. Amphiphilic block copolymers are most often composed of hydrophilic blocks covalently linked to hydrophobic ones. They have the ability to self-assemble in bulk or in solution, leading to different soft materials6 such as micelles, vesicles7, polymersomes8, and gels. The peculiar behavior of these copolymers in solution allows their use as surfactants, emulsifiers9, drug carriers10, etcBio-based amphiphilic polymers can be either totally natural and made of renewable species for both the hydrophilic and hydrophobic parts (e.g. alkyl polyglycosides11, nucleolipids12, polysaccharide-block-polypeptide13 and oligosaccharide linked to hydrophobized oligosaccharide14), or partially bio-sourced where one block is from renewable resources. Nowadays, this latter class is being widely developed with the synthesis of diblock copolymers based on oligosaccharides15, peptides16 or lipids17.Most vegetable oils are mainly composed of triglycerides, which are also known as triacylglycerols (TAG)s, with long alkyl chains (between 12 and 20 carbons). Vegetable oils and their derivatives (fatty alcohols, esters and acids) have been extensively investigated for the synthesis of oleochemical surfactants. These surfactants can be made ionic with the introduction of a negatively charged head, typically a sulfonate17 or carboxylate group18 (sulphonate of a glycerol ester or ester of a sulphated methylglucoside). Positively charged heads, typically quaternary ammonium or amphoteric species such as betains, can also be encountered. Moreover non-ionic surfactants can be produced by associating lipids with hydrophilic molecules like diethanolamine or with hydrophilic polymers such as poly(ethylene oxide) (PEO)9,17, poly(glycerol)19 or some poly(oxazoline)s: (poly(2-ethyl-2-oxazoline) or poly(2-methyl-2-oxazoline)). Furthermore, we note that a study of block-copolymers based on poly(2-methyl-2-oxazoline) or poly(2-ethyl-2-oxazoline) as the hydrophilic block and hydrophobic poly(2-oxazoline) synthesized from fatty acids has been recently reported20.In this work we focus on the synthesis of amphiphilic polymers composed of a natural lipidic hydrophobic part (a vegetable oil or its derivatives) and a hydrophilic chain based on poly(2-methyl-2-oxazoline), so called LipoPOx. Poly(2-methyl-2-oxazoline) is a more hydrophilic polymer than PEO21 and is used as a building block for various macromolecular architectures22. POx exhibits a low toxicity23 whereas some recent studies suspected toxicity for PEO resulting in bioaccumulation24. Thus poly(2-methyl-2-oxazoline) appears to be a good alternative to PEO-based polymers25. Few synthetic routes in obtaining LipoPOx with various structures have been described in the literature so far. First linear lipopolymers were synthesized using lipidic initiators such as iodoalkyl26, alkyl trifluoromethanesulfonate or alkyl tosylate27 initiators for the polymerization of MOx (2-methyl-2-oxazoline). Furthermore, multi-step strategies were developed to obtain pseudo-bicatenar lipopolymers based either on diacylglycerol or glyceroldiethers. In this case, the synthesis and the use of 1,2-didodecanoylpropyl-p-toluene sulfonate28 or 1,2-O-dioctadecyl-sn-glyceroltosylate or triflate29 as the macroinitiator for the polymerization of MOx can be one approach. The other pathway consists in the preparation of poly(2-methyl-2-oxazoline) and then coupling a lipidic block such as disteaorylphosphatidylethanolamine25c or 1,2-didodecanoylpropyl28. It should also be mention that a complex structure of lipopolymer was previously reported using a modified vegetable oil as the starting initiator for the synthesis of LipoPOx30. In this case castor oil was modified with p-toluenesulfonyl chloride to initiate the cationic ring-opening polymerization (CROP) of MOx.As opposed to previous reported work in the literature, our strategy was based on the chemical modification of double bonds of the triglycerides without modification of the triacylglycerol structure. The main objective and the novelty of this contribution is the extension of the synthesis of LipoPOx to any unsaturated vegetable oils and to all fatty esters. Our strategy is described in Scheme 1. Following to this route, unsaturated lipids were converted into lipidic alcohols thanks to the addition of 2-mercaptoethanol (ME) onto double bonds using the thiol-ene coupling (TEC) reaction. The resulting modified lipids were transformed into initiators for the polymerization of MOx. The strategy was first assessed using methyl oleate and afterwards applied to crude oil. We report here the ability of LipoPOx derived from fatty esters and triglycerides to self-organize in aqueous solution. It is important to point out that literature reported the self-organization of linear LipoPOx in water31 has been previously reported in the literature. In the present study, we were interested in the self-organization of branched LipoPOx based on crude oil and in the formation of nanoparticles.
Scheme 1 General synthetic route towards amphiphilic polymers LipoPOx, MO = Methyl oleate, GSO = Grapeseed oil, HMO = Hydroxylated methyl oleate, HGSO = Hydroxylated grapeseed oil, LipoPOx = lipopolyoxazoline (amphiphilic polymer).Experimental sectionMaterials 2-Methyl-2-oxazoline (MOx) was dried and distilled from CaH2 and stored under a dry nitrogen atmosphere. Ether from VWR, tetrahydrofuran (THF), acetonitrile (ACN) and ethyl acetate (EtOAc) from Carlo Erba, anhydrous dichloromethane and chloroform (CHCl3) from Sigma were distilled before use and stored under dry nitrogen. Grapeseed oil (GSO) (an usual commercially available oil), methyl oleate (MO) (purity 70%), 2,2-dimethoxy-2-phenylacetophenone (DMPA) (purity 99%), triethylamine (Et3N), N,N-benzyldimethylamine, pyridine, trifluoromethanesulfonic anhydride (Tf2O), potassium carbonate (K2CO3) and piperidine from Aldrich, 2-mercaptoethanol (ME) and sodium iodide (NaI) from Sigma, MgSO4 from VWR and p-toluenesulfonyl chloride (TsCl) and chloroacetyl chloride (CAC) from Fluka were used without further purification. Dialysis membranes Spectra/Por - MWCO 500-1000 were purchased from Spectrum Laboratories, Inc.CharacterizationNuclear magnetic resonance (NMR) spectra were recorded on a RMN Bruker Avance I 300 MHz or on a Bruker Avance III 600 MHz spectrometers. Chemical shifts (1H NMR) were referenced to the peak of residual CHCl3 at 7.26 ppm. Chemical shifts (13C NMR) were referenced to CDCl3 at 77 ppm. Fourier transform infrared (FTIR) spectra were recorded with a Perkin Elmer Spectrum 100 spectrometer equipped with an attenuated total reflectance (ATR) using a ZnSe crystal. The composition of crude oils was determined by gas chromatography (GC) analysis after conversion of the triglycerides into fatty acids (FA)s and methyl esters. The mixture was analyzed on an Agilent 6890 series using a Supelcowax 10 capillary column (SGE, Courtaboeuf, France): length, 30 m; internal diameter, 0.32 mm; film thickness, 0.25 m and carrier gas: helium at a flow rate of 20 ml/min, splitting ratio: 100, injector temperature: 250C, FID detector temperature: 270C. The temperature profile was: 185240C at 4C/min, 225C for 10 min. The HPLC/ESI system consisted of a capillary HPLC system (Alliance 2790, Waters) and an ESI source of time-of flight (TOF) mass spectr